University of Bristol  Explore Bristol Research. Early version, also known as preprint


 Clarence Wilkins
 1 years ago
 Views:
Transcription
1 Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), DOI: / Early version, also known as preprint Link to published version (if available): / Link to publication record in Explore Bristol Research PDFdocument The final version of this paper has been published in The final version of this paper has been published in the Journal of Composite Materials, Vol 40/Issue 14, July 2006 by SAGE Publications Ltd, All rights reserved. The Authors,2006. University of Bristol  Explore Bristol Research General rights This document is made available in accordance with publisher policies. Please cite only the published version using the reference above. Full terms of use are available:
2 NUMERICAL INVESTIGATION OF PROGRESSIVE DAMAGE AND THE EFFECT OF LAYUP IN NOTCHED TENSILE TESTS STEPHEN R. HALLETT AND MICHAEL R.WISNOM Department of Aerospace Engineering, University of Bristol, University Walk, BS8 1TR, UK SUMMARY: This paper presents results from a new approach to finite element modelling of notched damage in composite materials using interface elements to model intra and interply damage. The technique is used to examine and predict the failures observed in tensile, double edge notched specimens using four different layups made up from glass/epoxy prepreg. Due to the detailed modelling of the individual damage modes their interaction is well characterised. The analytical results obtained compare well with detailed test observations, capturing delamination and intraply splitting. By including the subcritical damage that occurs at the notch tip in the model, the stress singularity is removed and failure criteria can be used to predict ultimate ply failures. KEYWORDS: Notched strength, progressive damage, finite element analysis, interface element Author to whom correspondence should be addressed. tel: fax:
3 INTRODUCTION The subject of damage in notched composites is an area of extensive research. A highly detailed analysis is required to accurately predict stresses in the region of a notch tip 1,2. For sharp notches finite element analysis shows a stress singularity at the notch tip. This results in arbitrary values, which are dependent on mesh size, being predicted for the maximum stress in the load bearing plies. In reality the stress levels at which ultimate failure occurs are modified by the presence of progressive damage, which develops in the specimen from relatively low levels of applied load. This takes the form of splitting within the plies in the loading direction at the notch tip, matrix cracking transverse to the load and delamination between the plies. An experimental investigation by Kortschot and Beaumont 3 has provided a description of this damage and the failure patterns for crossply laminates. This has been extended to other layups by Hallett and Wisnom 4 and other authors 5,6,7. One approach to determine notched strength has been to use the point or average stress at a characteristic distance from the notch tip as proposed by Whitney and Nuismer 8. Many variations of such failure criteria have been put forward but a general short coming of such approaches is that they require experimentally determined parameters that are layup specific. Kortschot and Beaumont 9 have used finite element models with damage inserted at appropriate locations to obtain the relation between stress and damage and subsequently used this in expressions to predict how the damage will initiate and grow. An alternative approach is to include the damage prediction in the finite element model such as has been done by Chang and Chang 10, using a set of interactive failure criteria followed by property degradation to predict progressive damage growth and residual strength in open hole tension tests. Coats and Harris 6 have used a stress based progressive damage model to predict matrix cracking and 2
4 fibre failure. Delamination was not included and results were significantly mesh size dependant, however once this was calibrated against a single test result good predictions were obtained for residual strength of a centrally notched specimen over a range of specimen sizes and notch to width ratios. Methods such as these include the damage modelling in the continuum elements used to model the plies but do not explicitly take account of the splitting and delamination that occurs as subcritical damage. Kwon and Craugh 11 have included a thin delamination layer at the 0/90 interface of a notched crossply model that shows reasonable predictions for the shape of delamination. Iarve et al 12 have compared analytical predictions and experimental observations of the strain field at an open hole with an associated intraply split. This has shown that modelling of the split by property degradation of elements does not give good results. The physical discontinuity due to the ply split needs to be included in the model in order accurately predict the strain distribution. The interface element approach is one method of inserting a discontinuity into a finite element model. This approach has been developed largely to model delamination in composites 13,14,15. This technique has the advantage that it can be used to predict both the initiation and progression of the delamination. It does however require an apriori knowledge of the potential failure sites and elements to be inserted along such a path. Good results can be achieved for single and mixed mode loading and analyses have been correlated for example with end notch flexure (ENF), double cantilever beam (DCB) or mixed mode bending (MMB) tests 16. Previous work has used the interface element technique to predict both the delamination and splitting prior to ultimate failure 17 in crossply laminates. Here this has been extended and applied to four different layups. The effect of inclusion of subcritical damage in the model on 3
5 prediction of ultimate strength and failure mode by a simple strain based criterion has been examined. EXPERIMENTAL RESULTS Quasistatic tensile tests have been conducted using Hexcel Eglass/913 double edgenotched specimens. The results from these tests have been extensively reported in reference 4 and are only briefly summarised here. Scaled tests giving widths of 10, 20 and 40mm were performed for each layup. Of the available data, the 20mm wide specimens were chosen for comparison with the analytical results. The specimen geometry and layups tested are shown in Figure 1. The damage development was monitored from the start of loading and its growth was recorded using a digital video camera. Figure 2 shows some typical results from the 20mm wide specimens of all four layups tested. The images shown are not taken at regular time intervals but have rather been chosen to best show the damage development. Damage initiates at the notch tips in the form of clearly visible splits within each ply, extending in the fibre direction. This occurs at a relatively low stress compared to the ultimate failure load. Additional intraply matrix cracks develop transverse to the applied load in the central section. Adjacent to the splits are areas of delamination, seen as darker areas in Figure 2. The ultimate tensile strength of the specimen is controlled by fibre failure except in the case of the [45/90/45] s laminate where smaller specimens failed by delamination and fibre pullout only. 4
6 FINITE ELEMENT ANALYSIS Finite element analyses of the 20mm wide tests have been conducted using the explicit code LSDyna. The models were built up from stacked shell elements, with each ply within the laminate being modelled with a separate layer. Since each laminate is symmetric, only a half model through the thickness was used. To model delamination between the plies in the region of the notch, interface elements have been used, the formulation of which is described later in this paper. In order to connect the plies with interface elements it is required that adjacent plies have coincident nodes. It is therefore a quasi  two dimensional analysis which ignores through thickness tension and compression due to lack of offsets between the plies. This was felt to be an acceptable simplification since the delamination is primarily driven by shear. A linear elastic analysis has further been used to examine differences in fibre direction stresses between quasitwo dimensional shell and three dimensional brick models. Significant differences were not observed for thin laminates such as those examined here. Figure 3 shows a schematic view of a typical model ([+45/90/45/0] s layup) and boundary conditions together with interface element locations. In addition to the delamination damage between plies, splitting within each ply has been modelled using interface elements. Again coincident nodes are required and these have been inserted in each ply in a line extending from the notch tip in the fibre direction. Experimental work has shown this to be the predominant site of split locations. Without the inclusion of this subcritical damage, the stress state at the notch tip would form a singularity and hence the values obtained would be mesh dependent, making it difficult to incorporate failure criteria. The interface element approach overcomes this limitation and allows the detailed damage development to be included in the model using only elastic material properties, nonlinear shear behaviour, G Ic, G IIc and the matrix failure stress, all of which can be obtained experimentally. 5
7 Figure 4 shows experimental and numerical results of a 20mm wide crossply specimen all at 200MPa applied far field stress. Figure 4b shows the splitting and delamination damage predicted by failure of interface elements and Figure 4c shows the 0 fibre direction stress distribution. By comparison the fibre direction stress distribution in a model that has no interface element failure (Figure 4d) shows a highly localised stress concentration with a maximum value in excess of the unidirectional fibre failure stress 18. The subcritical damage clearly has an effect of blunting the notch, cause a redistribution of stress. This is significant for predicting failure of the load bearing plies since if stress or strain based criteria (as are commonly implemented in finite element codes) are used, the model without any subcritical damage will be predicted to fail at applied stress levels well below those observed in tests. The angle of the notch (θ) in the tests was 60. Analysis showed no difference in results between a sharp notch (θ = 0 as modelled in reference 17) and an angled notch as tested, since the subcritical damage modifies the stress field as soon as the split initiates. The angle of the notch in the modelling work presented here is for visualisation only and therefore 45 has been used in order to make it easier to preserve a regular mesh of mm in the area of interest. Since LSDyna is an explicit code it is better suited to modelling of dynamic events of very short duration. Quasistatic events can however be modelled if sufficient care is taken to ensure that dynamic effects are not significant. In order to ensure that the analysis completes in a reasonable time, a number of techniques are employed to reduce the CPU time taken. The analysis is run at a faster loading rate than the test, mass scaling is used to increase the timestep and damping is employed. The kinetic energy of the system is carefully monitored throughout to ensure that these changes have minimal effect. Additionally analyses 6
8 have been conducted at varying loading rates and levels of mass scaling to ensure results are not affected by these procedures. INTERFACE ELEMENTS AND SUBCRITICAL DAMAGE The interface element is essentially a 3 degree of freedom nonlinear spring with interaction between the degrees of freedom. The initial spring stiffness is calculated from an assumed resin rich layer 0.005mm thick, a nodal area calculated from the area of the shell elements attached to each node and a Young s modulus of 4GPa which is typical for epoxy resin. For ease of calculation a uniform element size has been used in the area of delamination and splitting. For the elements representing the delamination damage, only shear failure needs be considered since through thickness effects and hence mode I type failure are ignored. The shear properties of the element are assumed to be uniform in every direction on the shear plane and equivalent to a mode II type failure. The response of the interface element to an applied displacement can be seen in Figure 5a. The equivalent force  relative displacement response remains linear until a maximum is reached after which the slope is reduced such that the area under the curve is equal to the mode II fracture energy for the element concerned. The element is assumed to have failed when the force reaches zero. Previous work 17 used a perfectly plastic post yield behaviour instead of work softening. A study was done for both the work softening and perfectly plastic behaviour. Both analyses give similar results with the work softening behaviour leading to greater numerical stability since there is not a sudden reduction in force at each interface element failure. The maximum force for each element in the current analysis was calculated from a strength value of 75MPa 17. 7
9 For a crossply layup loaded orthogonally to the fibre directions it is sufficient to use the same one dimensional interface element for the intraply splitting as for the delamination since there is only mode II loading 17. In order to extend the analysis to layups other than crossply, mixed mode behaviour was included in the interface element. Mode I and mode II energy components are combined using equation 1 and failure occurs when the left hand side is equal to 1. GI GI G + G II C II C 1 Equation (1) The maximum force for the mixed mode case is based on the Von Mises yield criterion. The subject of mixed mode loading has been given much consideration in the literature with the majority of work being done on delamination. In the current model mixed mode loading occurs only in the splitting but this is thought to be very similar to delamination growth as both occur in the resin regions between fibres. After the Von Mises criterion is exceeded, the resultant force in the interface element is reduced such that equation 1 is satisfied. Figure 5b gives a graphical representation of the equivalent force  relative displacement behaviour of the interface element under mixed mode loading conditions. The mode ratio will not necessarily remain constant throughout the period of loading of a single interface element. If this changes, the area under the equivalent force  relative displacement curve (and hence the energy) is accounted for by adjusting the softening gradient. This allows for small changes in loading direction, ensuring the energy balance is maintained. It is not a completely general solution since once softening has initiated the force in the interface element cannot increase. It was felt to be adequate since large changes in mode ratio were not observed in individual interface elements. The mode ratio is of course 8
10 permitted to change as the split extends during damage development and different interface elements fail. Predicted damage has been compared to the test results in terms of split length and delamination location. Figure 6 shows that relatively good correlation has been achieved for growth of the 0 ply split in the crossply specimens. Correlation was found to be worst at the split initiation point. This may be due to residual stress from the curing process or machining defects from the cutting of the notch, which are not taken into account in the model. As the growth of the split progresses, the correlation improves. It can be seen that the analytical split growth rate is strongly dependent on the value of G IIc used. Due to previously discussed similarities in the damage process between splitting and delamination and difficulties in obtaining experimental data for the fracture energies is has been assumed sufficient to use the same data for both the splitting and delamination interface elements. Here two values taken from the literature have been used, 1.08N/mm (reference 19) and 0.9N/mm (using an average of the results presented for differing adjacent ply angles in reference 20), with the lower value giving better correlation for final split length. It is possible that using a single value for the fracture energy as the split grows is not sufficient and will cause a variation in correlation due to the Rcurve effect. Wisnom and Chang 17 found that it was necessary to include the nonlinear shear behaviour of the material in the model in order to achieve good correlation for the split growth. A piecewise linear curve fit to the data from reference 21 has been used here and is shown in Figure 7 together with a subset of the test data. G IC is not a critical value for the delamination or splitting in the crossply specimen but is required for splitting in the other laminates modelled. A value of 0.25N/mm 19 was used. The ply elastic material properties are shown in Table 1. 9
11 Figure 8 shows the subcritical damage results near to the mean experimental failure load from analyses for the different layups that were tested. Photographs of a typical 20mm wide specimen are shown at the same scale from a representative test at the same applied stress. For the crossply layup a half model was used. For those layups that contained ±45 fibres a full model was used since there is no true plane of symmetry due to the layup. It can be seen that there is generally good agreement in both the location and extent of delamination and splitting. Comparison with tests at exactly equivalent positions during loading is difficult due to the scatter in test data. In the experimental photographs it can be seen that in addition to the major splits starting from the notch tip there are a significant number of other matrix cracks in the laminates. Uniformly distributed matrix cracks have been reported as the site of delamination initiation 22. Experimental evidence suggests that for the notched case the significant delamination grows from the intraply splits associated with the notch tip. The matrix cracks observed in the material in the region between the notch tips do not have a significant effect on this delamination growth. In all of the layups damage initiated at the notch tip by splitting which agrees well with the experimental observations presented in reference 4. In order for the split to propagate in the fibre direction of each ply at least one of the delamination elements attached to the same nodes must also fail to allow relative displacement of the two split element nodes. Split growth rates in each of the 45, 90, 45 and 0 directions was not necessarily equal. Once the splits had started to propagate away from the notch tip into the specimen, triangular regions of delamination began to form between adjacent splits. These are shown in Figure 8 at the individual interfaces which when overlaid on top of each other combine to give the equivalent picture to that observed experimentally. 10
12 ULITIMATE FAILURE MODELLING The model described above was used to examine the final failure modes predicted when a ply failure criterion was introduced. Complete ply failure as a result of fibre failure was included by means of a quadratic criterion between fibre direction and shear response. This was implemented as a strain formulation (equation 2) in order to better take account of the nonlinear shear behaviour. Once this criterion is exceeded in a given element it is deleted from the analysis. ε ε γ12 + 1C γ12c 1 Equation (2) The fibre direction tensile failure strain (ε 1C ) was obtained from careful testing of UD specimens that were waisted in the thickness direction by dropping plies 23. A mean value of 3.5% was obtained for specimens with four and eight plies in the gauge length 18. A value of 5% was used for shear failure strain (γ 12C ) based on discussion in reference 21. It is arguable that the transverse matrix cracking as seen in Figure 2 will affect the formation of delamination and splitting but in the analyses conducted here it was not felt to be significant since initiation is controlled by the location of the notch tip. This was backed up by analyses in which the elastic transverse modulus was artificially reduced, no discernable difference in damage pattern could be observed. The stress distribution within each ply however was more strongly affected since its load bearing capacity is influenced by the development of the matrix cracks. The reduction factor was calculated from the observed matrix crack density of 30 cracks/cm in crossply tests 4 and an analysis developed by Kashtalyan and Soutis 24 which predicts a 15% reduction in laminate axial stiffness. This 11
13 requires approximately a 50% reduction in stiffness of the 90 plies from the value quoted in table 1. This reduced stiffness was not included in the previous analysis for subcritical damage since it did not affect the extent of splitting and delamination but has been included in analyses for ply failure. Looking only at the maximum applied far field stress at failure for the 20mm wide specimens it can be seen that there is relatively good agreement between test and analysis for the first three layups (Figure 9). The final layup shows worse correlation to test and this is attributed to the different failure mode that was observed in this layup compared to the others. Each layup analysed warrants further discussion with respect to the failure mode and its comparison to test. Figure 10 shows the final failure for the test and analysis of the crossply layup. The finite element result shows only a close up of the 0 ply with the failed elements removed (using equation 2). The experimental result shows all plies with the damage highlighted using strong backlighting. Ultimate failure in both the test and analysis occurs across the width of the specimen starting at the notch tip with failure of the 0 fibres. This rapidly progresses across the width of the specimen. The fibrefailure observed in tests is not exclusively orthogonal to the loading direction as can be seen in Figure 10, but progresses at an angle away from the notch tip, indicating an influence of shear stress. This is accompanied by additional splitting and delamination similar to that seen before the fibre failure. The model does not have the capacity to capture these further splits and this may be the cause of the differences in the failure patterns observed. The model takes account of the direct and shear stress interaction through the relationship in equation 2 and it is this interaction that causes the path of failed elements to progress in the fibre direction rather than directly across the specimen width. The 12
14 direction of fibre failure is somewhat different to that observed in test where it is at approximately 45 to the notch tip. Further work is required to investigate the detailed nature of the stress interaction in order to improve correlation. The test results for the [+45/90/45] s layup showed two possible failure modes. The first showed considerable amounts of delamination but the catastrophic failure of the specimen was due to failure of the fibres across the specimen width. The second mode was failure by delamination only and the plies pulling out from between each other without fibre failure. This can occur since there are no 0 plies in this layup. The first mode is captured well by the analysis and comparison with a test that exhibited this mode is shown in Figure 11. Tests on the [+45/90/45/0] s layup show fibre failure to occur across the width of the specimen and also some fibre pullout and some delamination back towards the specimen grips once the fibre failure has extended more than half way across the specimen width (Figure 12). The analysis predicts fibre failure in all plies in a band which closely approximates the area of failure observed. A slightly surprising result was the failure of the 90 ply by fibre failure in the finite element model as well as splitting in the fibre direction by failure of the interface elements (a site of potential splitting has been modelled starting from the notch tip). This has been confirmed to occur in the tests by thermal deply of the failed specimens which does indeed show some of the 90 plies to have failed in a very similar manner, initially splitting and then fibre failure at an angle to the fibre direction 4. Tests on the [+45/90/45/0 2 ] s layup showed a different failure pattern to that observed in the other layups. Only the internal 45 plies failed at the point of maximum load. On continuation of loading the central 0 plies separated from the adjacent plies by splitting and 13
15 delamination and continued to carry load until they failed by distributed fibre failure that was not affected by the position of the notch (Figure 13). Figure 14 shows that the analysis predicts fibre failure in the 45 ply but also in all of the other plies. This is possibly due to the fact that there is no capacity in the analysis to capture the distributed fibre failure that was observed in the tests. Additionally the extensive delamination back to the specimen grips was not predicted by the analysis although the damage prediction at 70% of the mean test failure load was reasonable (Figure 8). Once the subcritical damage has progressed a significant amount, the assumption of quasitwo dimensional behaviour may no longer be sufficient. Asymmetric sublaminates will be formed by the existence of the delamination and significant out of plane forces may develop which will contribute to further extension of the delamination and ultimate separation of the specimen. The analysis will under predict the amount of delamination since is does not take account of mode I opening of the delamination. The ultimate failure stress prediction for this layup (Figure 9) is somewhat below the mean test value, a result of the under prediction of the blunting effect caused by splitting and delamination. Correct prediction of the delamination may prevent premature ply failure. Work is ongoing to investigate the use of fully three dimensional models for the prediction of such delamination. MESH SENSITIVITY A significant problem with the modelling of material failure by finite element methods is that the resulting strength predictions can be dependent on the mesh size used. This makes the development of a general model that can be applied to different size specimens and different layups extremely difficult. A study was run on the [90/0] s layup in which the mesh size was 14
16 increased and decreased from the base analysis (0.25mm square mesh) to double and half its size. Examining only the ultimate failure stress it can be seen from Figure 15 that whilst there is some variation, all results are within 10% of the mean test result. However if the predicted subcritical damage is examined at the same applied stress level, as has been shown in Figure 16, it can be seen that the base and fine meshes are in good agreement but the coarse mesh has a considerably reduced damage area. There is an upper limit on the mesh size that can be used for the interface elements beyond which the damage will not propagate due to the high forces required for modelling the softening behaviour. The area of each interface element and hence the maximum force increases with the mesh size. At large sizes there is no longer sufficient stress concentration to initiate softening. This impedes the growth of the damage in the coarse mesh. The fact that the ultimate failure stress is reduced from that of the base mesh is due to the reduced amount of splitting and hence notch blunting that occurs. The good agreement between the base and fine meshes in Figure 16 indicates that once this threshold has been passed, mesh size dependencies are greatly reduced for the subcritical damage prediction. Similar behaviour has been observed in other interface element studies 25 with coarser meshes requiring greater applied loads for propagation due to the reduced number of elements in the cohesive zone. The reduction in ultimate failure stress from the base mesh to the fine mesh indicates that there is still a small mesh dependency in the ply failure prediction. This mesh dependency is however considerably less significant than if the subcritical damage had not been included in the model. 15
17 DISCUSSION An analysis technique has been successfully developed that predicts the detailed development of subcritical damage in notched laminates for layups that include ±45 plies. The effect of this damage on the stress distribution and final failure due to the inclusion of a ply failure criterion has been examined. The approach closely represents the physical mechanisms observed in the tests, and is able to predict failure of different layups from a single set of material properties that can be obtained from independent tests. The one layup that was an exception to this, [+45/90/45/0 2 ] s, exceeds the quasitwo dimensional assumptions made and exhibited a failure mechanism which thus far has not been included in the model. Mesh size has been shown to not be a significant issue for failure of the interface elements below a critical mesh size. The inclusion of the subcritical damage reduces the stress singularity at the notch tip and allows the use of a ply failure criterion but does not completely eliminate mesh size effects for the failure of the continuum elements. Examination of the final failure of the test specimens indicate that in some cases the analysis over predicts the amount of fibre failure. Whilst the assumption of mode II only delamination is sufficient when considering damage during its early stages of development it may not be adequate once the delamination has progressed sufficiently far such that the laminate is divided into two asymmetric sublaminates. This will cause a mode I contribution to the delamination. An additional failure mode which has not been considered is the further splitting in the plies once fibre failure has started to occur. This will have a similar effect to the initial notch blunting and inhibit the progression of fibre failure in the plies. Both of these mechanisms will have an effect on the ultimate failure modes and the fibre failure that is predicted. Whilst the current model adequately predicts the early stages of subcritical damage development these mechanisms 16
18 may have to be included to increase the ability to predict a greater range of failures in more complex laminates and loading scenarios. CONCLUSION It can be seen that the model presented gives an accurate description of the main failure modes prior to fibre failure, i.e. delamination and ply splitting, for a number of different layups and good correlation to test is achieved. In the case of the fourth layup this is limited to early stages of loading prior to the major delamination extending back to the grips. The damage has been modelled using only measured elastic material properties and fracture energies. A site of potential splitting and delamination does have to be assumed and interface elements inserted but their failure is predictive in nature. The importance of being able to model this damage is in the effect it has on the stress concentrations in the material. The splitting has an effect of blunting the notch which in turn affects the ultimate load carrying capacity of the material. This gives an improved accuracy to the finite element model for predicting ply failure since without this effect, failure would be significantly under predicted. The main focus of this work has been the inclusion of the different damage modes that contribute to the ultimate failure. The final notched strength of an individual layup is dependent on the damage mechanisms that occur and their interaction, which have been modelled in detail. There is an equally complex interaction of stresses and the individual components have been predicted with greater accuracy due to the included damage. This work has been funded by the U.K. Engineering and Physical Sciences Research Council under grant no. GR/N
19 LIST OF FIGURES Figure 1 Figure 2 Figure 3 Figure 4 Specimen geometry Typical results from the different layups tested Schematic view of finite element model (a) Experimental damage, (b) predicted damage, (c) 0 stress distribution with damage, and (d) stresses without damage modelling, all at 200MPa applied far field stress Figure 5 Equivalent force  relative displacement response for interface elements (a) mode II (b) mixed mode Figure 6 Figure 7 Figure 8 Split growth rate for crossply specimen Test data from reference 21 and piecewise linear fit used in the analysis Results for delamination and split location for different layups tested and modelled Figure 9 Figure 10 Figure 11 Figure 12 Figure 13 Ultimate failure stress for 20mm wide specimens test to analysis correlation Failure of the 20mm wide crossply specimen Failure of the 20mm wide [+45/90/45] s specimen showing fibre failure 20mm wide [+45/90/45/0] s layup analysis and test failure mode comparison Photograph of 40mm wide [+45/90/45/0 2 ] s specimen showing distributed failure 4 Figure 14 Figure 15 Figure 16 Failure pattern for the [+45/90/45/0 2 ] s layup 20mm wide specimen Failure stress for [90/0] s layup for different mesh sizes Effect of varying the mesh size 18
20 TABLES E 11 E 22 G GPa 15.4 GPa 4.34 GPa υ Table 1 Elastic material properties for eglass/913 19
21 REFERENCES 1 Kwon, S.W. and Sun, C.T. (2000) Characteristics of threedimensional stress fields in plates with a throughthethickness crack, International Journal of Fracture, 104: Hu, F.Z., Soutis, C. and Edge, E.C. (1997) Interlaminar stresses in composite laminates with a circular hole, Composite Structures, 37: Kortschot, M.T. and Beaumont, P.W.R. (1990) Damage mechanics of composite materials I: Measurements of damage strength, Composites Science and Technology, 39: Hallett, S.R. and Wisnom, M.R. (2005), Experimental investigation of progressive damage and the effect of layup in notched tensile tests, Journal Of Composite Materials, In press 5 Spearing, S.M., Beaumont, P.W.R. and Ashby, M.F. (1992) Fatigue damage mechanics of composite materials II: A damage growth model, Composites Science and Technology, 44(2); Coats, T.W. and Harris, C.E. (1999) A progressive damage methodology for residual strength predictions of notched composite panels, Journal of Composite Materials, 33(23);
22 7 Harris, C.E. and Morris, D.H. (1985) Role of delamination and damage development on the strength of thick notched laminates, Delamination and debonding of materials, ASTM STP 876; Whitney, J.M. and Nuismer, R.J. (1974) Stress fracture criteria for laminated composites containing stress concentrations, Journal of Composite. Materials, 8: Kortschot, M.T. and Beaumont, P.W.R. (1990) Damage mechanics of composite materials II: A damagebased notch strength model, Composites Science and Technology, 39: Chang, F.K. and Chang, K.Y. (1987) A progressive damage model for laminated composites containing stress concentrations, Journal of Composite Materials, 21; Kwon, K.Y. and Craugh, L.E. (2001) Progressive failure modelling on notched crossply fibrous composites, Applied Composite Materials, 8; Iarve, E.V., Mollenhauer, D. and Kim, R. (2003) Threedimensional modeling and experimental investigation of damage accumulation in open hole composite laminates, ICCM14, San Diego 13 Allix, O. and Ladeveze, P. (1992) Interlaminar interface modelling for the prediction of delamination, Composite Structures, 22:
23 14 Borg, R., Nilsson, L. and Simonsson, K. (2001) Simulation of delamination in fiber composites with discrete cohesive failure model, Composites Science and Technology, 61: Camanho, P.P., Davila, C.G. and De Moura, M.F. (2003) Numerical simulation of mixedmode progressive delamination in composite materials, Journal of Composite Materials, 37: Borg, R., Nilsson, L. and Simonsson, K. (2004) Simulating DCB, ENF and MMB experiments using shell elements and a cohesive zone model, Composites Science and Technology, 64; Wisnom, M.R. and Chang, F.K. (2000) Modeling of splitting and delamination in notched crossply laminates, Composites Science and Technology, 60: Khan, B., Potter, K., Hallett, S.R. and Wisnom, M.R. (2004) Size effects in unidirectional composites and quasiisotropic specimens in tension, 2 nd International Conference on Composites Testing and Model Identification, Bristol 19 Petrossian, Z. and Wisnom, M.R. (1998) Prediction of delamination initiation and growth from discontinuous plies using interface elements, Composites: Part A, 29: Shi, Y.B., Hull, D. and Price, J.N. (1993) Mode II fracture of+/ angled laminate interfaces, Composites Science and Technology, 47:
24 21 Wisnom, M.R. (1994) The effect of fibre rotation in +45 degree tension tests on measured shear properties, Composites, 26(1): Takeda, N. and Ogihara, S. (1994) Initiation and growth of delamination from the tips of transverse cracks in CFRP crossply laminates, Composites Science and Technology, 52: Khan, B., Potter, K. and Wisnom, M.R. (2005) Suppression of delamination at Ply Drops in Tapered Composites by Ply Chamfering, Journal of Composite Materials, In press 24 Kashtalyan, M. and Soutis, C. (2000) Stiffness degradation in crossply laminates damaged by transverse cracking and splitting, Composites: Part A 31: Turon, A., Dávila, C.G., Camanho, P.P. and Costa, J. (2005) An engineering solution for using coarse meshes in the simulation of delamination with cohesive zone models, NASA Technical Memorandum
25 FIGURES θ W=20mm a 50mm end tabs [90/0] s [+45/90/45] s [+45/90/45/0] s [+45/90/45/0 2 ] s L = 100mm 2a/w = 0.5 θ = 60 Figure 1 Specimen geometry 24
26 Figure 2 Typical results from the different layups tested 25
27 Figure 3 Schematic view of finite element model 26
28 Figure 4 (a) Experimental damage, (b) predicted damage, (c) 0 stress distribution with damage, and (d) stresses without damage modelling, all at 200MPa applied far field stress 11 27
29 Figure 5 Equivalent force  relative displacement response for interface elements (a) mode II (b) mixed mode 28
30 2.5 2 L/a Applied Stress (MPa) Test Data 4 G IIc =0.9N/mm G IIc =1.08N/mm Figure 6 Split growth rate for crossply specimen 29
31 Shear Stress (MPa) Test data Piecewise linear fit Shear Strain (%) Figure 7 Test data from reference 21 and piecewise linear fit used in the analysis a 30
32 Figure 8 Results for delamination and split location for different layups tested and modelled 31
33 Applied Stress (MPa) Test Analysis 50 0 [90/0] s [45/90/45] s [45/90/45/0] s [45/90/45/0 2 ] s Layup Figure 9 Ultimate failure stress for 20mm wide specimens test to analysis correlation 32
34 Specimen centreline 0 Analysis Figure 10 Failure of the 20mm wide crossply specimen 33
35 Figure 11 Failure of the 20mm wide [+45/90/45] s specimen showing fibre failure Figure 12 20mm wide [+45/90/45/0] s layup analysis and test failure mode comparison 34
36 Figure 13 Photograph of 40mm wide [+45/90/45/0 2 ] s specimen showing distributed failure Figure 14 Failure pattern for the [+45/90/45/0 2 ] s layup 20mm wide specimen 35
37 Applied Stress (MPa) Test Mean Fine Mesh Base Mesh Coarse Mesh Figure 15 Failure stress for [90/0] s layup for different mesh sizes 36
38 Figure 16 Effect of varying the mesh size 37
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationFREE EDGE DELAMINATION ONSET CRITERION
FREE EGE ELAMINATION ONSET CRITERION G. MARION now, 2, formerl 3, R. HARRY 2, and F. LECUYER MEYSYS, 29 rue J. Rostand, 9873 ORSAY CEEX, FRANCE 2 Laboratoire de Génie Mécanique, IUT Bordeaux I, 3345 TALENCE
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationAcoustic emission analysis for failure identification in composite materials
Acoustic emission analysis for failure identification in composite materials Markus G. R. Sause Experimental Physics II Institute of Physics University of Augsburg 1. Motivation 2. Methods of AE analysis
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationUniversity of Bristol  Explore Bristol Research. Publisher's PDF, also known as Version of record License (if available): Unspecified
Garza Rodriguez, C., Smith, D., Shterenlikht, A., & Pavier, M. (2015). Advances in the deep hole drilling technique for the residual stress measurement in composite laminates. In Proc 5th Thematic Conf.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationDiscrete ply modelling of open hole tensile tests
Discrete ply modelling of open hole tensile tests Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol To cite this version: Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol.
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationDamage analysis of composite structures: a software editor point of view and illustration on industrial applications
1 SAMCEF Solver group, SAMTECH s.a., A Siemens Company 2 Aerospace & Mechanical Engineering Dpt, University of Liège Damage analysis of composite structures: a software editor point of view and illustration
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationAnálisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas
San Miguel de Tucuman, Argentina September 14 th, 2011 Seminary on Análisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas Antonio Caggiano 1, Guillermo Etse 2, Enzo
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationPractical methodology for inclusion of uplift and pore pressures in analysis of concrete dams
Practical methodology for inclusion of uplift and pore pressures in analysis of concrete dams Michael McKay 1 and Francisco Lopez 2 1 Dams Engineer, GHD Pty 2 Principal Dams/Structural Engineer, GHD Pty
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationTHE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES
Powder Metallurgy Progress, Vol.3 (003), No 3 119 THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES A.S. Wronski, A.Cias Abstract It is wellrecognized that the
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationCohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
University of Liège Aerospace & Mechanical Engineering Cohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
More informationMixedMode Decohesion Finite Elements for the Simulation of Delamination in Composite Materials
NASA/TM2002211737 MixedMode Decohesion Finite Elements for the Simulation of Delamination in Composite Materials Pedro P. Camanho University of Porto, Porto, Portugal Carlos G. Dávila Langley Research
More informationNumerical simulation the bottom structures. grounding test by LSDYNA
5 th European LSDYNA Users Conference Methods and Techniques (3) Numerical simulation the bottom structures grounding test by LSDYNA Ainian Zhang Graduate School of Frontier Sciences, The University
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationFinite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation
Copyright 2013 Tech Science Press CMC, vol.35, no.1, pp.6785, 2013 Finite Element Analysis of Delamination in Woven Composites under QuasiStatic Indentation M. C. Song 1, B.V. Sankar 1, G. Subhash 1,
More informationDELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE
DELAMINATION IN MODE I AND II OF CARBON FIBRE COMPOSITE MATERIALS : FIBRE ORIENTATION INFLUENCE F. LACHAUD 1,2, R. PIQUET 2, L. MICHEL 1 2 LMT, IUT de énie Mécanique, 50, Chemin des Maraîchers, 31077 TOULOUSE
More informationDynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites
Engineering Fracture Mechanics 7 (5) 53 558 www.elsevier.com/locate/engfracmech Dynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites Sylvanus
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationPLATE GIRDERS II. Load. Web plate Welds A Longitudinal elevation. Fig. 1 A typical Plate Girder
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationINFLUENCE OF FLANGE STIFFNESS ON DUCTILITY BEHAVIOUR OF PLATE GIRDER
International Journal of Civil Structural 6 Environmental And Infrastructure Engineering Research Vol.1, Issue.1 (2011) 115 TJPRC Pvt. Ltd.,. INFLUENCE OF FLANGE STIFFNESS ON DUCTILITY BEHAVIOUR OF PLATE
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More information